Presentation on theme: "EXPLOSIVE WELDING OF LARGE-SIZE TITANIUM– STEEL SHEETS: INFLUENCE OF AMBIENT GAS А. А. Berdychenko, L. B. Pervukhin, and O. L. Pervukhina TUBULAR ITEMS."— Presentation transcript:
EXPLOSIVE WELDING OF LARGE-SIZE TITANIUM– STEEL SHEETS: INFLUENCE OF AMBIENT GAS А. А. Berdychenko, L. B. Pervukhin, and O. L. Pervukhina TUBULAR ITEMS EXPLOCLAD WITH Ti O. L. Pervukhina, I.V.Saikov and L. B. Pervukhin Influence of explosion welding technology parameters on the titanium structure 2010
Report plan 1. Influence of ambient gas in technological gap on the titanium structure. 2. Features titanium structure at its volume deformation defined by the size of welding gap.
1 Explosive; 2 electric detonator; 3 titanium clad plate, thickness is 5 mm; 4 titanium bar, thickness is 5 mm; 5 titanium base plate, thickness is 5 mm. Research methods TEM, X-ray, laser mass- spectograph 1 electric detonator; 2 explosive; 3 clad plate ; 4 base plate ; 5 starting sensor; 6 shutdown sensor of the fist frequency meter; 7 shutdown sensor of the second frequency meter; 8 connecting cables; 9 frequency meters; 10 power supply Research technique 2
Air D=3940 - 1880 m/s Change of concentration of oxygen С О (а) и nitrogen С N (б) in metal of vortical zones 1 V к =3980 m/s; 2 V к =2640 m/s; 3 V к =1880 m/s. 3 V к =3980 m/s. V к =1880 m/s.
D=2690 м/с Nitrogen Oxygen Change of gas (Сг) concentration in a material of vortical zones of welded connections received in the environment of oxygen (1) and nitrogen (2) 4
D=2690 м/с Argon Helium Welding in the environment of inert gases of argon and helium considerably improves structure of welded joint, raises its plasticity and stabilizes quality of welded joint along the full area regardless of its sizes. The best quality and stability of properties provides with filling of technological gap with helium. 5
The technology of large-size two-layer sheets (Steel + Titanium) manufacture by explosion welding was developed and patented. The technical conditions “Two-layer intermediates Steel+Titanium produced by explosion welding” were formalized and conformed to Gosatomnadzor. Trumpet lattices of condensers are produced from two-layer clad in OAO «Kaluga turbine factory ». 8 Ti+Steel
The beginning of process 2800 mm from the beginning of welding process Microstructure Steel 10 + Titanium ВТ1-0 welded by explosion in argon atmosphere. 7 Ti+Steel Grade of bimetal, sizes, mm Durability of joint, MPa Tests, degree Tearing offShearBendLateral bend More 80
Problems at manufacture of long-length cylindrical copper - titanium details by explosion welding : 1. Instability of process at length over 250 mm 2. Occurrence of cracks in clad layer; 3. Formation of intermetallic phases and titanium into a joint zone. Choice of technological gap size : - Thermodynamic conditions of qualitative joint formation (temperature, pressure, time) must be provided. - It is necessary to exclude conditions of deformation localization in the titanium and cracks formation. - It is necessary to take into account the possible fluctuation of technological gap in the limits with length of units. 9
Deformation features of a titanium pipe at explosive compression Experiments spent on cylinders from titanium pipe with the size of grain 25 microns. Length of 70 mm, external 20 mm, internal 11 mm 10 Explosive titanium steel
Titanium microstructure at different deformations after shock-wave loading.1 Development of a localization strip The size of grain Critical parameter of localization
1.To except cracks formation in Ti the size of technological gap should provide the relative volumetric cylinder deformation no more than 0,22. 2. To quench a deformation localization in Ti it is necessary to provide heating of the surface layer to the temperature of plastic state. Clad long-length copper bars by a titanium pipe 3. To save the thermodynamic conditions of explosion welding it is necessary to except titanium burning in a gap by means of its filling with inert gas. 1212 1- Copper core 2 - titanium pipe 3 - The top cover 4 - The bottom cover 5 - Technological gap 6 - Explosive 7 - Sand 8 - Detonator
r =0.1 r =0.6. Intermediate Ti+Cu for a contact jaw r =0.6. Change of deformation mechanism of titanium during explosive loading is revealed Copper bar 25 mm, l = 1000 mm Titanium pipe wall thickness is 2.5 mm The relation of length to diameter = 33 Titanium deformation on the end sites of intermediates 1313
The experimental technology of long-length Ti+Cu bars manufacture by explosion welding providing 100% joint continuity and necessary electrical resistance of joint zone was developed under the research of deformation features of titanium pipe and influence of ambient gas in the welding gap. Conclusion: 1414